Formation of coordination polymer glass by mechanical milling: dependence on metal ions and molecular doping for H<sup>+</sup> conductivity.
Ohara, Yuki; Hinokimoto, Akira; Chen, Wenqian; Kitao, Takashi; Nishiyama, Yusuke; Hong, You-Lee; Kitagawa, Susumu; Horike, Satoshi; Chemical communications (Cambridge, England) 54 (2018) 6859–6862; doi:10.1039/c8cc02399a

data_7121598
_publ_section_title
;
 Formation of coordination polymer glass by mechanical milling: dependence
 on metal ions and molecular doping for H<sup>+</sup> conductivity.
;
_journal_issue                   50
_journal_name_full
'Chemical communications (Cambridge, England)'
_journal_page_first              6859
_journal_page_last               6862
_journal_paper_doi               10.1039/c8cc02399a
_journal_volume                  54
_journal_year                    2018
_chemical_formula_moiety         'C2 H5 Co0.5 N3 O4 P'
_chemical_formula_sum            'C2 H5 Co0.5 N3 O4 P'
_chemical_formula_weight         195.52
_chemical_name_systematic        CoTz
_space_group_crystal_system      orthorhombic
_space_group_IT_number           60
_space_group_name_Hall           '-P 2n 2ab'
_space_group_name_H-M_alt        'P b c n'
_symmetry_space_group_name_Hall  '-P 2n 2ab'
_symmetry_space_group_name_H-M   'P b c n'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2018-03-19
_audit_creation_method
;
Olex2 1.2
(compiled 2017.08.10 svn.r3458 for OlexSys, GUI svn.r5381)
;
_audit_update_record
;
2018-03-19 deposited with the CCDC.
2018-04-30 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.477(3)
_cell_length_b                   9.531(3)
_cell_length_c                   15.479(5)
_cell_measurement_reflns_used    3710
_cell_measurement_temperature    223.15
_cell_measurement_theta_max      27.4623
_cell_measurement_theta_min      3.2162
_cell_volume                     1250.6(7)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      223.15
_diffrn_detector_area_resol_mean 28.5714
_diffrn_measured_fraction_theta_full 0.984
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'Saturn724+ (4x4 bin mode)'
_diffrn_measurement_method       dtprofit.ref
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0337
_diffrn_reflns_av_unetI/netI     0.0182
_diffrn_reflns_Laue_measured_fraction_full 0.984
_diffrn_reflns_Laue_measured_fraction_max 0.987
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            8989
_diffrn_reflns_point_group_measured_fraction_full 0.984
_diffrn_reflns_point_group_measured_fraction_max 0.987
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.492
_diffrn_reflns_theta_min         3.216
_diffrn_source_current           40.0000
_diffrn_source_power             2.0000
_diffrn_source_voltage           50.0000
_exptl_absorpt_coefficient_mu    1.682
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.9302
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            orange
_exptl_crystal_colour_primary    orange
_exptl_crystal_density_diffrn    2.077
_exptl_crystal_description       prism
_exptl_crystal_F_000             788
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.2
_refine_diff_density_max         0.314
_refine_diff_density_min         -0.358
_refine_diff_density_rms         0.068
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.085
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     135
_refine_ls_number_reflns         1421
_refine_ls_number_restraints     198
_refine_ls_restrained_S_all      1.038
_refine_ls_R_factor_all          0.0271
_refine_ls_R_factor_gt           0.0256
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0373P)^2^+0.9725P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0669
_refine_ls_wR_factor_ref         0.0681
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1359
_reflns_number_total             1421
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8cc02399a2.cif
_cod_data_source_block           CoTz
_cod_depositor_comments
'Adding full bibliography for 7121595--7121598.cif.'
_cod_original_cell_volume        1250.7(7)
_cod_original_formula_sum        'C2 H5 Co0.50 N3 O4 P'
_cod_database_code               7121598
_shelx_shelxl_version_number     2018/1
_shelx_estimated_absorpt_t_max   0.730
_shelx_estimated_absorpt_t_min   0.730
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups, All N(H) groups
 At 1.5 times of:
  All O(H) groups
2. Restrained distances
 N1-C1 = C1-N3 = N3-C2 = C2-N2 = N2-N1
 1.34 with sigma of 0.02
 N3A-C1 = C1-N1A = N1A-N2A = N2A-C2A = C2A-N3A
 1.34 with sigma of 0.02
 N1-N3 = C1-C2 = N3-N2 = C2-N1 = N2-C1
 2.2 with sigma of 0.04
 N3A-N1A = C1-N2A = N1A-C2A = N2A-N3A = C2A-C1
 2.2 with sigma of 0.04
3. Restrained planarity
 N1, N3, N2, C1, C2
 with sigma of 0.01
 N3A, N1A, C2A, C1, N2A
 with sigma of 0.01
4. Uiso/Uaniso restraints and constraints
N1 \\sim N3 \\sim N2 \\sim C1 \\sim C2 \\sim N3A \\sim N1A \\sim C2A \\sim C1
\\sim N2A: within 2A with sigma of 0.001 and sigma for terminal atoms of 0.002
Uanis(N1) \\sim Ueq, Uanis(N3) \\sim Ueq, Uanis(N2) \\sim Ueq, Uanis(C1) \\sim
Ueq, Uanis(C2) \\sim Ueq, Uanis(N3A) \\sim Ueq, Uanis(N1A) \\sim Ueq,
Uanis(C2A) \\sim Ueq, Uanis(C1) \\sim Ueq, Uanis(N2A) \\sim Ueq: with sigma of
0.001 and sigma for terminal atoms of 0.002
5. Others
 Sof(H1B)=Sof(N1A)=Sof(N2A)=Sof(H2AA)=Sof(C2A)=Sof(H2AB)=Sof(N3A)=1-FVAR(1)
 Sof(N3)=Sof(N1)=Sof(N2)=Sof(H2)=Sof(C2)=Sof(H2A)=Sof(H1A)=FVAR(1)
6.a Aromatic/amide H refined with riding coordinates:
 N2(H2), C2(H2A), C1(H1A), C1(H1B), N2A(H2AA), C2A(H2AB)
6.b Idealised tetrahedral OH refined as rotating group:
 O4(H4), O3(H3)
;
_shelx_res_checksum              63892
_olex2_submission_special_instructions 'No special instructions were received'